The role of photonics in energy
Zakya H. Kafafi,a,
* Raúl J. Martín-Palma,b
Ana F. Nogueira,c
Deirdre M. O ’Carroll,d
Jeremy J. Pietron,e
Ifor D. W. Samuel,f
and Loucas Tsakalakosh
aLehigh University, Center for Photonics and Nanoelectronics, Department of Electrical and Computer Engineering, Bethlehem, Pennsylvania 18015, United States
bUniversidad Autónoma de Madrid, Departamento de Física Aplicada, Cantoblanco, Madrid 28049, Spain
cUniversity of Campinas, Laboratório de Nanotecnologia e Energia Solar, Campinas-SP 13083970, Brazil
dRutgers University, Department of Materials Science and Engineering, Department of Chemistry and Chemical Biology and IAMDN, Piscataway, New Jersey 08854, United States
eSurface Chemistry Branch, Code 6170, Naval Research Laboratory, Washington, DC 20375, United States
fUniversity of St Andrews, Organic Semiconductor Centre, SUPA, School of Physics and Astronomy, St. Andrews, Fife KY16 9SS, United Kingdom
gNorth Carolina State University, Department of Materials Science and Engineering, Raleigh, North Carolina 27695, United States
hGeneral Electric–Global Research Center, Electrical Technologies and Systems, Micro and Nano Structures Technologies, Photonics Laboratory, Niskayuna,
New York 12309, United States
Abstract. In celebration of the 2015 International Year of Light, we highlight major break- throughs in photonics for energy conversion and conservation. The section on energy conversion discusses the role of light in solar light harvesting for electrical and thermal power generation;
chemical energy conversion and fuel generation; as well as photonic sensors for energy appli- cations. The section on energy conservation focuses on solid-state lighting, flat-panel displays, and optical communications and interconnects.© 2015 Society of Photo-Optical Instrumentation Engineers (SPIE) [DOI:10.1117/1.JPE.5.050997]
Keywords: chemical energy conversion; dye sensitized cells; electrical energy conversion;
energy; energy conservation; energy conversion; flat panel displays; International Year of Light; light management; light-emitting diodes; optical communications; optical interconnects;
optoelectronics; organic light-emitting diodes; organic photovoltaics; organic-inorganic hybrid cells; perovskite solar cells; photocatalysis; photoelectrochemical solar cells; photonic crystals;
photonics; photovoltaics; plasmonics; sensors; solar cells; solar fuels; solar harvesting; solid- state lighting; sun-tracking systems; thermal energy conversion; water-splitting.
Paper 15040V received May 9, 2015; accepted for publication Aug. 3, 2015; published online Oct. 12, 2015.
1 Historical Background
The most comprehensive ancient account of the science of light is a millennium old, dating from the Islamic golden age when the Arab scholar Ibn al-Haytham (Alhazen) composed and published his seminal seven-volume Book on Optics. It was nearly 700 years later that Christiaan Huygens developed a wave theory of light, while Newton proposed a corpuscular (particle) theory of light.
Authors are listed alphabetically.
*Address all correspondence to: Zakya H. Kafafi, E-mail:firstname.lastname@example.org; Raúl J. Martín-Palma, E-mail:email@example.com;
Ana Flávia Nogueira, E-mail:firstname.lastname@example.org; Deirdre M. O’Carroll, E-mail:email@example.com; Jeremy J. Pietron, E-mail: firstname.lastname@example.org; Ifor D. W. Samuel, E-mail: email@example.com; Franky So, E-mail: firstname.lastname@example.org;
Nelson Tansu, E-mail:email@example.com; and Loucas Tsakalakos, E-mail:firstname.lastname@example.org 1947-7988/2015/$25.00 © 2015 SPIE
In his book, A Dynamical Theory of the Electromagnetic Field, Maxwell mathematically unified light, electricity, and magnetism.1This modern theory of light is only 150 years old!
These great milestones were followed by the work of Einstein,2who introduced the concept of photons to explain photoelectric effect data in terms of light energy being carried in discrete, quantized packets. He demonstrated that only photons with a certain threshold frequency (energy) impinged upon a metal surface can cause the ejection of electrons. The discovery of the law of this photoelectric effect was a foundation of the quantum revolution and was the primary reason for the Nobel Prize awarded to Einstein in 1922.3
A recent and elegant demonstration of light’s dual nature was reported by the group of Carbone at École Polytechnique Fédérale de Lausanne (EPFL) in Switzerland, who captured a snapshot of the concurrent behavior of light as both a wave and a stream of particles4(Fig.1).
Understanding the quantum nature of light and electrons was crucial to the discovery of other phenomena that involve the interaction of light with electric charges, such as the photoconduc- tive effect, i.e., photoconductivity, the photovoltaic (PV) effect, and the photoelectrochemical (PEC) effect.
In this paper, we will review some of the enabling photonic technologies that followed based on last century’s fundamental discoveries related to the interaction of light and matter.
Section 1 gives an overview of the role that photonics plays in power generation through electrical, thermal, and chemical energy conversion, as well as in sensor technology.
Section2 describes technological advances where photonics is important for energy conser- vation. It covers solid-state lighting, flat-panel displays, and optical communications and interconnects. Advances in photonics such as the development of the worldwide optical com- munications network that carried the news of Charles Kao’s receiving the Nobel Prize in 2009,5thanks to his proposal 50 years ago to use optical fibers to transmit phone calls across great distances, will be highlighted. Other examples will include the revolution in solid-state lighting that earned Isamu Akasaki, Hiroshi Amano, and Shuji Nakamura the Nobel Prize in Physics in 2014.6This award was based on their development of efficient blue light-emitting diodes (LEDs), enabling bright and energy-saving white light sources. This work was pre- ceded by the seminal work of R. N. Hall et al.7on diode lasers, as well as that of Holonyak and Bevacqua8and Allen and Grimmeiss,9who developed red LEDs in the early 1960s, and that of Round10 and Losev,11who reported electroluminescence from carborundum early in the 20th century. The 21st century witnessed another revolution in display technology with the development and commercialization of flat-panel displays. The technology on which these
Fig. 1 Energy-space photography of light confined on a nanowire simultaneously shows both spatial interference and energy quantization.4
flat-panel displays is based will soon undergo another transformation with the introduction of bright, efficient, and stable organic light-emitting diodes (OLEDs).
2 Role of Photonics in Energy Conversion
The sun supplies the energy that allows all life on earth. The enormous power of the sun can be used in three main ways. The first is the conversion of sunlight to electrical power, which is discussed in Sec.2.1. The second is the conversion of sunlight to thermal power, which is briefly described in Sec.2.2. The third is the conversion of sunlight directly to fuels, which is the topic of Sec.2.3. In addition, the role of photonic sensors in energy harvesting and the production of power are covered in Sec.2.4.
2.1 Solar Light Harvesting and Electrical Energy Conversion
Most solar cells on rooftops now convert sunlight into electricity using the PV effect first dem- onstrated by Becquerel.12With the advent of the silicon PV cell in 1954,13humankind increas- ingly found ways of using semiconductors for many energy conversion applications. Among the first applications of solar PVs was their use in space to power control systems and other critical functions on space vehicles.14This subsequently grew into the application of PVs in residential solar systems for off-grid applications and has matured into grid-connected residential systems and solar power plants in the last 15 years.15The progress in solar PVs in terms of cell power conversion efficiencies (PCEs) can be seen in the chart from the (US) National Renewable Energy Laboratory (NREL) shown in Fig. 2. NREL makes certified measurements of PV cells, and the chart shows how different solar PV technologies have developed as a function of time (for small-area, champion solar cells). As will be explained below, the highest efficiency technologies are accompanied by very high cost and complexity, so the dominant solar cells are in the middle of the efficiency range. The newest technologies are at the bottom right of the chart, but their rapid rate of development and efficiency improvement could make them the solar PV technologies of the future. In a single-junction solar cell, the amount of light absorbed and the maximum voltage obtainable both depend on the bandgap of the semiconductor. This leads to a trade-off between the amount of light absorbed and the open-circuit voltage. The theoretical limit for the PCE of a single-junction PV cell under AM1.5 irradiation is calculated to be 33.7%
using the detailed balance theory developed by Shockley and Queisser in 196116and taking into account thermalization losses and low-bandgap losses in the solar cell.
2.1.1 Inorganic solar cells
The most important commercially available PV materials systems today are based on inorganic semiconductors. The vast majority of solar modules are based on silicon, which is the second most abundant material in the earth’s crust, hence, these modules are of relatively low cost. The record silicon solar cell efficiency is 25.6%. Modules with a PCE of∼21%, fabricated by apply- ing a thin film of amorphous silicon-based heterojunction to a silicon surface, are commercially available.18The majority of commercial Si modules have PCEs in the range of 14% to 18%. The modules are typically fabricated by manufacturing Si wafers with the correct doping level to form a p–n junction, along with suitable front and back contact (typically screen-printed).
Both single-crystalline and multi/polycrystalline wafers are used in the industry. The cells are then laid out on a backing sheet and strung together with metal tabs. An adhesive layer is applied to bond the front glass cover, ensuring that good edge moisture barriers are also in place. Photonics plays an important role in Si-based solar cells and modules since it is an indirect bandgap semiconductor and hence has a relatively long absorption depth across the solar spectrum. Most importantly, light-trapping structures must be fashioned on the front sur- face of the wafers to ensure that long wavelength light is adequately trapped within the solar cell and is not lost from reflection at the back contact and subsequent impingement on the front surface (within the escape cone). Light trapping is typically achieved by etching the front surface of the wafers to form a random texture or by an anisotropic etch that forms pyramidal structures on the Si surface.19Another important photonic aspect of Si modules is related to the optical
losses that can occur at the glass/adhesive interface, as well as at the glass to air interface due to reflection. Significant advances to minimize such optical losses have been made over the last two decades.20Further discussion of these topics is found in Sec.2.1.3.
Another commercially important class of materials is based on inorganic thin films, primarily related to the CdTe21and CuðIn; GaÞSe2(CIGS) materials systems.22CdTe solar cell efficiencies have been reported at 19.6% and CIGS at 20.5%. Until recently, thin-film solar cells have been lower in cost than Si solar cells due to the fact that they are direct bandgap semiconductors, and hence, a very thin layer (typically 1 to 5 μm) can be deposited using low-cost deposition proc- esses directly onto a large-area glass substrate. This significantly lowers the manufacturing cost.
One can use the glass growth substrate as the window layer, or can use it as a backing layer and add another glass window layer. In both cases, it is possible to manage the light using suitable antireflective coatings (ARC, see below).23Today Si and CdTe-based modules are competitive in cost (typically measured in $/Watt).
III–V semiconductor materials are also important for high-efficiency PV conversion. GaAs cells have reached 1 Sun efficiencies of 28.8%, and multijunction III–V cells have achieved an efficiency of 37.9% at 1 Sun.18Figure2gives a summary of the record efficiencies achieved by these different PV cells over the last few decades. III–V solar cells have been reserved for spe- cialty applications, primarily for space due to their exceptionally high cost (ca. three orders of magnitude higher cost per square meter than Si). This high cost is due to several factors, includ- ing the low abundance of group III and V elements, the high expense of growing III–V crystals, the lack of a good diffusion process for forming the p–n junction (an epitaxial layer is needed), the need for another surface passivation layer to minimize surface recombination, and the need for expensive materials/processes to form good Ohmic contacts. An ARC is also always needed on the III–V surface. On the other hand, the high efficiency of III–V solar cells/modules is attrib- uted to the direct bandgap nature of these semiconductors, which implies a short absorption depth as well as a high charge carrier mobility and high minority carrier lifetimes due to the low nonradiative losses that occur in the crystal. Surface recombination is readily minimized in III–V cell technologies by applying a suitable passivation layer. Another advantage is the fact that the bandgap of 1.5 eV gives the optimal balance of absorption of the solar spectrum and open-circuit voltage. Photon recycling in III–V solar cells has been critical in improving their performance and led to a record PCE of 28.8% for a single-junction cell.24Recent efforts to produce lower-cost III–V modules have allowed penetration into previously unattainable markets.25,26
The state-of-the-art high-performance inorganic solar cells technology is primarily pursued using multijunction stacked tandem solar cells.27Using materials with different bandgaps that overlap with the visible and near-IR solar spectral region leads to the absorption of photons over a wide range of energies with a small loss of photon-to-electrical energy conversion, thereby overcoming the Shockley–Queisser limit. Tandem structures require the development of appro- priate absorber materials and the matching of the current density throughout all the stacked layers. Progress has been made using primarily III–V multijunction tandem cells with record efficiencies of 44.4% under concentration (302 Suns) for InGaP/GaAs/InGaAs solar multijunc- tion cells.27Recent work has reported the superior lasing characteristics of GaInNAs quantum well lasers with very low threshold.28–30By taking advantage of this progress, the integration of III–V multijunction cells with GaInNAs-containing alloys as one of the cell materials has enabled a record PCE of 43.5%.31Other materials including InGaN32and InN33are currently being pursued, while others such as GaAsBi34are being considered for multijunction solar cells.
One way of improving the cost-effectiveness of these very expensive but highly efficient solar cells is to use a concentrator, i.e., to harvest light over a large area but deliver it to small but very efficient solar cells35 (e.g., planar Fresnel lenses36).
Another recent development deals with the application of various nanostructures to produce novel architectures for solar cells and, in some cases, to take advantage of new energy conversion physics. If classes of nanostructures are considered by their dimensionality, zero-dimensional quantum dots (QDs) have been applied to building new solar cell architectures that utilize quan- tum confinement in unique ways. For example, Green et al.37have proposed an all-silicon QD tandem device and are making progress toward the fabrication of such structures.38QDs have also been applied as novel photonic coatings that take advantage of either up- or downconversion
of portions of the solar energy spectrum in order to more effectively use bands that are lost due to thermalization or due to being sub-bandgap (and hence not absorbed).39One-dimensional (1-D) nanostructures, such as inorganic nanowires and carbon nanotubes, have also been explored in various novel device architectures. For example, silicon nanowires and III–V nanowire solar cells have been demonstrated40–42 and show promise for producing low-cost, high-efficiency, flexible solar cells.43Two-dimensional (2-D) quantum well nanostructures have been employed to convert near-IR photons and, hence, boost the efficiency of III–V solar cells.44 Finally, three-dimensional inorganic nanoarchitectures have been fabricated and show promising cell performance.45
2.1.2 Organic and hybrid solar cells
As depicted in Fig.2 and discussed above, PV cells based on crystalline inorganic semicon- ductors have reached impressive PCEs of> 28% in single-junction and 38% in multijunction device architectures under full-sun illumination.46However, this class of PV cells suffers from high production and energy costs, which result in long financial and energy payback times.47 This drawback has fostered the development of a new generation of solution-processable solar cells,48–50which benefit from low-cost materials (e.g., organic molecular and polymeric materi- als), high-throughput manufacturing methods, such as reel-to-reel coating, and low-energy expenditure.51This new class of PVs is referred to as emerging PV cells and can be categorized according to the materials used and mechanisms invoked: PEC or dye-sensitized solar cells (DSSCs), organic (molecular and polymer) solar cells, hybrid organic–inorganic solar cells, and QD solar cells. An overview of these emerging and promising technologies is given with the best cell PCEs achieved so far appearing at the bottom right of the NREL chart shown in Fig.2. Since they are relatively new compared to their inorganic counterparts, it is not surprising that their efficiencies are much lower than those of the most established inorganic solar cells. However, the slope of their PCEs has been quite steep over the last few years, especially for the promising PV technology based on organic–inorganic hybrid materials (e.g., perovskites).
DSSCs, also known as PEC cells, were the first emerging PV technology to reach acceptable efficiency values. Consequently, DSSC research has initially attracted the largest number of researchers and the largest amount of industry cooperation, as well as the largest number of solar panel prototypes and related products. Since the first demonstration in 1991 by O’Regan and Graetzel,52 and after two decades of research and development, DSSCs with an iodine/tri-iodide (I−∕I3−) liquid electrolyte have achieved light to electric PCEs of > 11%
using ruthenium dyes,53> 12% based on zinc porphyrin dyes,54and> 10% based on metal-free organic dyes.55 Recently, through the molecular engineering of zinc porphyrin sensitizers, Grätzel and coworkers have reported solar cells with 13% PCE. The new sensitizers feature the prototypical structure of a donor–π-bridge–acceptor, maximize electrolyte compatibility, and improve light-harvesting properties.56 Using SM315 dye with the cobalt (II/III) redox shuttle resulted in DSSCs that exhibit a high open-circuit voltage (VOC) of 0.91 V, short-circuit current density (JSC) of 18.1 mA cm−2, and a fill factor (FF) of 0.78. However, there are several problems that limit the mass production and long-term stability of such devices, such as leakage and evaporation of the liquid electrolyte, and corrosion of the metal-based current collectors (silver, copper, etc.) by iodine. As a result, substantial effort has been made to find alternative electrolytes and/or introduce new concepts to develop electrolyte-free DSSCs. In solid-state DSSCs (ss-DSSCs), the liquid electrolyte is entirely replaced by a solid organic hole transport material (HTM). For the solid-state version (ss-DSSC), PCEs > 20% have been predicted,57 using low-cost materials,58low temperature processing (< 150°C), and reel-to-reel fabrication methods.59,60
Organic (molecular and polymeric) solar cells represent another and different category in the class of emerging PVs. These solid-state devices have attracted a lot of attention in the last 20 years as one of the most promising technologies for low-cost solar energy conversion.
A key difference from their inorganic semiconductor counterparts results from their low dielec- tric constant and gives rise to strongly bound upon solar light absorption at room temperature.
A chemical potential is required between the hole (p-type) transporter/electron donor and the electron (n-type) transporter/acceptor in order to separate the photogenerated carrier charges and
often involves the use of a strong electron acceptor. One subclass of these devices is based on a light-harvesting material that consists of a mixture of a conjugated polymer as the p-type material or hole transporter/electron donor and a fullerene derivative as the n-type material or electron transporter/acceptor. The operating mechanism in these organic solar cells, discovered in the mid-1990s by Sariciftci et al.,61is based on photoinduced electron transfer from a conducting polymer such as a poly(p-phenylene vinylene) (PPV) derivative to a fullerene derivative. This finding opened up a very rich and intensive research field involving the synthesis of new con- jugated polymers and copolymers with low-bandgap and high charge carrier mobilities, novel fullerene derivatives with better solubility, morphology control of the active light-harvesting layer, and different solar cell configurations. In particular, the so-called bulk heterojunction (BHJ) in which the donor and acceptor are mixed together is most widely used because it enables efficient charge generation even in materials with very limited exciton diffusion length. Further refinements included novel contact materials aiming to give better interfaces for electron and hole collection, and the investigation of ground and excited states to understand the complex mechanisms involving exciton formation and diffusion, charge-transfer state formation and separation followed by charge transport and collection.
Organic solar cells with BHJ architectures using conducting polymers and fullerene mole- cules are by far the most studied,62,63achieving PCEs close to 10% using one polymer as an absorber (i.e., single-junction devices), in both regular and inverted device structures.64–67The chemical nature of the electron donor polymers has evolved from simple structures, such as PPV and poly(3-hexylthiophene) (P3HT), to more complex copolymers specially designed to have both electron donor and acceptor groups in their structures in order to reduce their bandgap. One example is the newly synthesized narrow-bandgap semiconducting polymer poly [[2,6′-4,8-di(5- ethylhexylthienyl)benzo[1,2-b;3,3-b] dithiophene] [3-fluoro-2[(2-ethylhexyl)carbonyl]thieno [3,4-b]thiophenediyl]], which when used in the light-harvesting layer led to a very efficient cell that delivered a certified PCE of 9.94%.67Recently, Yang and coworkers have fabricated a multijunction solar cell having a PCE exceeding 11%, suggesting great potential for tandem architectures in organic photovoltaic (OPV) research68(see Fig. 3).
Small molecules offer some advantages over conducting polymers, such as synthetic flex- ibility, ease of purification, less batch-to-batch variation in properties, higher hole and electron mobilities in some cases, and intrinsic monodispersity. Efficient molecular BHJ solar cells have recently been reported in which merocyanine dyes, squaraine dyes, fused acenes, triphenyl- amine, benzofuran benzothiadiazole, diketopyrrolopyrrole, benzodithiophene, and other chro- mophores, such as oligothiophenes and push-pull organic dyes, have been employed as the
Fig. 3 (a)J − V characteristics and (b) action spectra, external quantum efficiency as a function of wavelength, for single-junction photovoltaic (PV) cells based on poly(3-hexylthiophene):ICBA, PTB:[6,6]-phenyl-C71 butyric acid methyl ester (PC71BM), and LBG∶PC71BM as the active light- harvesting layers. (c) J − V characteristics and (d) device configurations (front subcell/back subcell) of inverted double-junction tandem OPVs. (Reproduced with permission from Ref.68
© 2014 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim.)
light-harvesting donor components.69–71 State-of-the-art OPV devices achieved PCEs up to 10%.72–75 Recently, molecular OPVs based on oligothiophenes with five thiophene units in the backbone and 2-(1,1-dicyanomethylene)rhodanine as end capping units exhibited a PCE of 10%.76
State-of-the-art solution-processed devices generally rely on the BHJ of polymer electron donors and fullerene electron acceptors.77Fullerene derivatives, such as [6,6]-phenyl-C61butyric acid methyl ester (PC61BM) and [6,6]-phenyl-C71 butyric acid methyl ester (PC71BM), have played a leading role as electron acceptor materials; however, they suffer from poor absorption in the visible and near-IR regions. Recently, nonfullerene electron-accepting chro- mophores, such as perylene diimide, naphthalene diimide, vinazene, fluoranthene-fused imide, benzothiadiazole, rhodanine, and diketopyrrolopyrrole, have been incorporated with success in BHJ molecular and polymeric solar cells.78–84 So far, state-of-the-art BHJ devices based on nonfullerene acceptors have shown PCE up to 6%.84
Hybrid organic–inorganic solar cells have structures similar to the cells described above where the electron-accepting fullerenes are substituted with inorganic semiconductors (e.g., TiO2, ZnO, CuInS2, PbS, CdSe, and CdTe) nanoparticles.85–88 Chalcogenide nanoparticles with quantum confinement properties have also been considered and used as sensitizers in DSSCs.89,90 These solar cells offer a series of advantages over the more traditional BHJ OPVs based on the polymer/fullerene systems. Some of the expected advantages are (1) a con- tribution to light absorption by an inorganic acceptor can lead to the generation of more photo- carriers, due to their larger linear absorption coefficients compared to those of fullerene derivatives; (2) the absorption of nanoparticles can be tuned to cover a broad solar spectral range, as a result of modification of their size and shape, complementary to that of the organic electron donor/hole transporter; (3) the physical dimensions of some inorganic semiconductors can be tailored to produce 1-D nanostructures, to allow efficient exciton dissociation, i.e., charge separation and electron transporting pathways simultaneously; (4) ultrafast and efficient photo- induced charge carrier transfer between the electron acceptor (inorganic nanoparticles) and the electron donor (the organic semiconductor); (5) the acceptors have relatively high electron mobility; and (6) good photo- and chemical stability.91 However, to date, PCEs achieved for hybrid organic–inorganic solar cells are significantly lower than those of OPV devices, which is primarily due to the challenges in controlling the interface between the nanoparticles and the polymer, and achieving a well-defined matrix with a continuous percolation network.
Furthermore, the presence of surface traps on the nanoparticles can be problematic for achieving good charge generation and carrier transport. An efficiency of 3.5% has been achieved in a BHJ architecture when combining CdSe nanorods and PbS QDs with different polymers.92,93 More recently, silicon and an organic polymer (e.g., P3HT) and carbon nanotubes have been combined to give hybrid solar cells with efficiencies reaching 11%.94,95
A recent breakthrough occurred in the last couple of years with the demonstration of highly efficient solar cells based on organic/inorganic lead halide perovskite absorbers. These light-har- vesting organic–inorganic materials have transformed the field of organic/inorganic hybrid PV devices.96,97Solution processed PVs incorporating perovskite absorbers, such as CH3NH3PbI3 and CH3NH3PbI3−xClx, have achieved efficiencies of 20.1% (certified, but not stabilized) in solid-state device configurations, surpassing liquid DSSCs, evaporated and tandem organic solar cells, as well as various thin-film inorganic PVs, thus establishing perovskite-based solar cells as a robust candidate for expanding the worldwide PV market. In 2009, hybrid per- ovskites were first used in the work of Kojima et al.98as the sensitizer (absorber) in a DSSC with liquid electrolyte, generating only a 3.8% efficiency. The breakthrough, however, came in 2012 when the group of Snaith at the University of Oxford and the group of Grätzel at EPFL combined the perovskite with the well-known DSSC solid-state HTM, 2,2′,7,7′-tetrakis(N,N-di-p-methox- yphenyl-amine)-9,9′-spirobifluorene (spiro-OMeTAD).99,100 The Oxford group demonstrated that a mesoporous TiO2 scaffold is not necessary and that the hybrid perovskites are able to transport both electrons and holes. In subsequent reports, efficiency values of 15% were attained in different systems with various morphologies, either in nanoheterojunction or planar thin-film configurations with different chemical compositions and preparation routes.101–106To date, effi- ciency values exceeding 16% have been reported with two quite different configurations, using CH3NH3PbI3perovskite in a classical solid-state DSSC and in a thin-film planar configuration
with CH3NH3PbI3−xClx, as shown in Fig.4.107,108The use of a mixed solvent ofγ-butyrolactone and dimethylsulfoxide followed by toluene drop-casting leads to solar cells with a certified PCE of 16.2% and no reported hysteresis.109The lack of hysteresis, which had been an obstacle for the stable operation of perovskite devices, was observed recently using thin films of organo- metallic perovskites with millimeter-scale crystalline grains with efficiencies close to 18%.110 Stabilization of the perovskite phase based on formamidinium lead iodide (FAPbI3) with meth- ylammonium lead bromide (MAPbBr3) as the light-harvesting unit in a bilayer PV architecture improved the PCE of the solar cell to> 18%.111Interestingly, electron transport layer-free and hole transport layer-free perovskite solar cells have also been reported, simplifying the device structure, thus opening up an interesting route to low-cost production of solar cells.112–114
The excellent PCEs achieved for solar cells based on perovskites are attributed to their long extended electron–hole diffusion length (> 1 μm),116,117broad solar light absorption (visible to near-IR), good solubility in organic media, and high carrier mobility. However, identifying the basic working mechanisms, which are still being debated, improving film quality, and improving device stability are important challenges that need to be addressed before serious consideration for their future development and commercialization.
Colloidal QD thin-film solar cells (CQD cells), depicted in Fig.5, are also part of the newly emerging PV technology. These devices have the potential to reduce manufacturing costs due to their solution processability, light weight, and being amenable to large area deposition. CQDs can be utilized in Schottky,118,119p–n heterojunction,120,121hybrid BHJ,91and as the sensitizers in PEC solar cells.122CQDs are nanometer-sized particles that are below the Bohr exciton radius of the specified material. CQDs are synthesized by rapid injection of the reactant into the reaction medium with stabilizing agents under an inert gas atmosphere. The role of the stabilizing agent, such as oleic acid and oleylamine, is to control growth rate, particle size, and dispersion of
Fig. 5 (a) Schematic diagram and (b) cross-sectional scanning electron micrograph (SEM) of a colloidal quantum dot (CQD)-based organic photovoltaic device with a PbS CQD film and TiO2∕ZnO junction. (Reprinted with permission from Ref. 118 © 2012 Macmillan Publishers, Ltd: Nature Nanotechnology.)
Fig. 4 (a) Mesoscopic perovskite solar cell with mesoporous TiO2layer and (b) planar structure without a mesoporous TiO2layer. Thin film on fluorine-doped tin oxide (FTO) is an n-type semi- conductor. HTM stands for hole transporting material. In the mesoscopic structure, electrons can be collected directly and/or via TiO2 layer. (Reproduced with permission from Ref. 115
© 2014 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim.)
the QDs. However, it may hinder the route for high-efficiency CQD-based PVs. The reduction of the interparticle spacing and passivation of surface traps in CQDs remain as primary challenges.
Among several candidates, PbS CQDs are of interest due to their ease of bandgap tunability in the visible region, and their simple, high-yield synthesis. Sargent122 and McDaniel et al.123 showed that performing a hybrid ligand exchange (long organic ligands are replaced simulta- neously by short ligands and by halide ions, e.g., CdCl2) results in efficient CQD solar cells in a p:n configuration with metal oxides (TiO2, ZnO). The PCE was improved to 8.5% by reducing the TiO2 thickness layer to 10 nm in order to increase the depletion width.124 As CQD and perovskite solar cells develop further, their environmental impact will need to be considered, leading to a search for lead and cadmium free materials.
2.1.3 Light management in solar cells
An essential function of photonics is to optimize light coupling into PV device and to improve light trapping within the absorbing light-harvesting layer. Since solar power converters primarily rely on inorganic semiconductors, there is a significant discontinuity in the refractive index between air or the encapsulant material, and the silicon or other inorganic semiconductors, such as III–V (e.g., GaAs, InP, etc.) and II–VI (e.g., CdTe) compounds—the discontinuity in the refractive index can be as high as 4.125This refractive index discontinuity leads to sig- nificant Fresnel reflection losses at the interface across the solar spectrum that can reduce the performance (i.e., PCE and energy yield) of the solar energy conversion system. It should also be noted that, in reality, a PV module consists not only of the semiconductor device, but also of various protecting layers, such as glass and protective/adhesive transparent polymers, and hence, the full module must be considered as an optical system when designing proper light-manage- ment approaches.20,126
The most widely used photonic method for minimizing reflection losses from the semicon- ductor surface is the single-layer or double-layer ARC.127These coatings are typically designed to minimize the reflection via interference of optical plane waves and consist of thin, transparent films of silicon nitride, silicon oxide, titanium oxide, and other similar compounds. Of course, it is possible to design more advanced multilayered ARCs to further minimize reflection losses;
however, for solar PV applications, this is typically too costly to implement. It is noted that such ARCs are deployed directly on the active solar cell and are then embedded within the polymer adhesive used to bind the protective glass cover for the solar module. Note that the glass itself, being a dielectric in the UV to near-IR portion of the solar spectrum, has a much lower refractive index than silicon, and hence, the outer module reflection loss is lower, i.e., ca. 4% reflection loss. Nevertheless, in recent years, glass manufacturers have also started to implement ARCs on the outer surface of the module, which, of course, provides additional requirements on the durability of the coating from mechanical handling during manufacturing and installation to environmental effects in the field, such as erosion.128
As the solar industry expanded rapidly in the last decade, it became apparent that thin-film ARCs have limitations with regard to their performance. This has to do with the fact that the reflection is often minimized for only a select region of the solar spectrum and also has a strong dependence on the angle of incidence. The surface reflectance increases rapidly as sunlight goes from normal incidence to high angles that arise during the morning and evening hours, which can lead to significant (up to ca. 30%) energy production losses.129One solution is to have an active system that tracks the sun (see Sec.2.4.1), but such systems are expensive and complicated, so passive systems that reduce these losses are of considerable interest. In recent years, the appli- cation of nanostructured surfaces (e.g., micro- or nanopillars or nanowires) that can be used to minimize reflection across the full solar spectrum and also up to high angles has been explored to address this problem.130,131These structures typically produce a graded effective refractive index that leads to an ultralow, broadband reflection that is also omnidirectional; hence, these struc- tures have been categorized as being omnidirectional antireflective (ODAR) layers.132A related concept has been to develop ODAR layers that can also act as downconverting layers, hence better optimizing the spectrum that the semiconductor absorbs to avoid thermalization losses when high-energy photons are absorbed.133
Indeed, downconversion is part of a broader light-management strategy being investigated by researchers worldwide to more effectively utilize the solar spectrum. High-energy (short wave- length) photons lead to thermalization losses when charge carriers are excited above the con- duction band edge. Alternatively, low-energy photons (long wavelengths) are not absorbed by the semiconductor and, hence, also lead to losses with respect to what the PCE of the solar cell could be if these photons were properly utilized. Calculations have shown that the limiting effi- ciency of a single-junction solar cell could go from 30.9% to 39.6% using a downconverting (or so-called quantum cutting) layer on the surface of the solar cell, whereas using an upconverting layer on the backside of the solar cell can increase the limiting efficiency (under 1 Sun illumi- nation) to 47.6%.134,135Research has focused on developing new optically active materials that can achieve up- or downconversion (e.g., QDs).38,136
In addition to minimizing surface and interface reflections, light-trapping methods have become important as the light-harvesting active layers have become thinner over the past few decades (thicknesses are approaching a few tens of microns for silicon-based solar cells;
are on the order of a micron or less for thin-film inorganic solar cells; and are in the region of 10 to 100 nm for organic solar cells). When the semiconductor active layers become thinner, material costs are reduced and, in some cases, the electrical properties are improved (e.g., due to reduced bulk electron–hole recombination). However, the optical density of the active layer is reduced and in-coupled solar radiation may not be fully absorbed during the first (or second) pass of light through the material. Therefore, methods to trap or increase the path length of light within the semiconductor layer have been developed to increase the effective optical density of the material.137,138 The use of highly reflective back electrodes, textured back reflectors or electrodes, and textured semiconductor surfaces has been found to improve light trapping and, hence, the PCE in a host of PV devices. However, there is a limit (known as the ergodic or light-trapping limit) to the number of passes that light can take within a thin-film active layer using textured surfaces or back reflectors, which is proportional to 4n2.139,140Approaches have been demonstrated that break this limit over relatively narrow wavelength ranges using photonic crystals (PCs), dielectric micro and nanostructures, and other photonic and plasmonic nanostruc- tures.141 For light trapping over the broad solar spectrum in thin-film PVs, texturing of back reflectors and semiconductor surfaces is still the most practical approach. Besides light trapping, for semiconductor materials with fast radiative recombination rates [high internal quantum effi- ciencies (QEs)], such as GaAs, photon recycling by means of highly reflective back electrodes and controlling interference effects within the active layer have enabled record single-junction solar cell PCEs.26,142,143
With the development of thin-film optoelectronic devices that have active layer thicknesses below the diffraction limit (i.e., <∼300 nm); such as small molecule and polymeric OPVs in which the active light harvesting layer thickness ranges from∼10 to 40 nm and up to ∼250 nm, respectively, light-management techniques using nanophotonic structures, particularly metallic plasmonic structures, have emerged.144–156Metal nanoparticles and structured metallic thin films can localize incident light to subwavelength dimensions due to the excitation of surface plas- mons—collective electron oscillations of the free electrons at the surface of metals. However, for such effects to be strong, the metals must exhibit weak intra and interband electronic absorption losses. Therefore, noble metals are typically used for subwavelength thin-film light management using plasmonics. However, even noble metals behave as nonideal metals at optical frequencies;
therefore, parasitic absorption loss is always present to some degree. Despite these losses, well- designed plasmonic nanostructures can greatly improve light harvesting for a range of energy applications that employ very thin layers or small absorber material volumes.
For example, arrays of discrete plasmonic nanoparticles and nanoantennas have been shown to effectively harvest and localize incident light within semiconductor thin films and, therefore, improve light absorption and electron–hole pair generation rate at the nanoscale. Far-field scat- tering by such nanostructures placed on top of or within thin-film PV devices have been shown to improve short-circuit current densities by∼20% to 70% (compared to analogous devices without the plasmonic nanostructures) through the increased effective path length of incident solar radi- ation with the semiconductor absorber layer.145–151Optimization of the albedo (ratio of scattering crosssection to extinction cross-section), location, degree of shadowing, and shape of the nano- structures is typically required to achieve significant improvements in short-circuit current
density. In addition to far-field scattering, near-field localization or trapping of incident light into guided surface plasmon polariton modes at the metal/semiconductor interface using nanostruc- tured metal electrodes, such as nanotextured or nanopatterned metal thin films and metasurfaces, is also of interest for increasing the effective absorption depth of semiconductor thin films.
Additionally, (semi)transparent metal nanowire arrays and nanohole arrays can both facilitate light trapping and in-coupling to guided surface plasmon polariton modes and also act as trans- parent electrodes.148,157–161Near-field localization using the aforementioned structures and using plasmonic nanoantenna structures has also been found to increase the generation rate of elec- tron–hole pairs, which can lead to increased PCE in thin-film PV devices. More recently, photo- sensitization of wide-bandgap semiconductors and generation and collection of hot electrons on plasmonic nanostructures were shown to be an alternative means to harvest solar energy for applications in PVs, photocatalysis, and solar-to-fuel energy conversion.152,162–164 Plasmonic absorber materials have also been considered for light harvesting without the need for semicon- ductor materials.165,166
2.2 Solar Light Harvesting and Thermal Energy Conversion
An important alternative to converting sunlight to electricity is to harvest the thermal energy directly where photonics also plays an important role. One simple application involves the use of concentrated solar power, where sunlight is focused onto long pipes coated with an opti- cally absorbing material and filled with a high-thermal capacity fluid, which is used to drive a turbine.167,168 From a photonics perspective, the emphasis has been on the development of advanced coatings with high absorption coefficients in the UV to the IR solar spectral region, which included the development of carbon nanotube and metallic nanowire arrays,169,170as well as PCs,171 with the goal to create nearly perfect black absorbers. The solar thermal concept has also been applied to a vertical configuration in which a circular array of mirrors is used to concentrate reflected sunlight onto a solar tower that uses heat to generate electricity.172 More commonly, sunlight is widely used (without concentration) for domestic water heating.
The progress made in solar PVs has enabled relatively efficient conversion of solar photons into electrons for electricity generation. In addition, it has opened up an interesting alternative way of converting thermal energy into electrical energy, namely thermophotovoltaics (TPVs).
The basic principle of a TPV system, illustrated in Fig.6, lies in heat supplied to an emitter leading to the emission of thermal radiation (photons). Thermally generated photons of sufficient energy are then absorbed in the TPV cell leading to the generation of electrons and holes, just as in a conventional PV device.173 A filter/reflector is used to transmit only photons of energy greater than the bandgap of the TPV cell and reflect lower-energy photons back onto the emitter so that their heat is recycled. The design of such a system involves optimizing three key com- ponents, where the first one is the heat source, which serves as the thermal blackbody radiation emitter. By identifying the temperature of the emitter, the peak wavelength of the blackbody radiation can be obtained, which in turn defines the choice of the semiconductor for the TPV cell. The filter/reflector needs to be designed to match the spectral properties of the emitter
DC power Emitter Filter / reflector TPV cell
Waste heat Heat
Fig. 6 Schematic of thermophotovoltaic systems including emitters, filter, and absorber PV materials.
and the TPV cell. This is achieved using PCs or multilayer structures where one can design a long-pass filter with precise sets of cut-off wavelengths.
The key applications of TPVs include the space station, cars, and heavy industries. The ther- mal radiation of interest has a temperature operation around 1000 to 1500 K, which corresponds to cut-off wavelengths of∼2 to 3 μm. For ensuring the stability of the emitters, the TPVemitters are commonly based on rare earth oxides, silicon carbide, and tungsten. In order to harness the thermal energy, the materials of interest for the TPV devices are based on inorganic semicon- ductors, such as Si and III–Valloys. More specifically, the use of GaSb and InGaAsSb is of great interest since their bandgaps can be tuned over the wavelength range of interest.174Such state-of- the-art materials (e.g., GaSb) are used with antireflection-coated tungsten foil on alumina design for the emitter in TPVs with an electrical efficiency of 10.6%.175 Progress in GaSb and InGaAsSb lasers176has also fueled tremendous improvement in the quality of materials relevant to the TPV applications. In addition, recent work on both dilute-nitride and dilute-SbN material systems has shown promise to push into the wavelength regime for TPV,177–180where the use of dilute-bismuthide materials as absorbers in the 2 to 3 μm spectral region has shown promise.181 For the emitter, a 2-D tantalum PC has been used, and an electrical efficiency up to 16% is predicted.182Another approach employs a graded-index tungsten emitter structure to enhance the spectral efficiency in the solar TPV system.183Future advances will result from the develop- ment of materials and the structure design of the emitters, filters, and PV cells to optimize the radiant efficiency and spectral and infra-red photon to electron conversion efficiencies of the PV cells in the TPV systems.
Thermoelectric materials offer an alternative approach to harness thermal energy by conver- sion of heat into electricity using the Seebeck effect.184Recent work has focused on nanostruc- tures and alloys to improve the thermal energy conversion in thermoelectric systems.185–189
2.3 Solar Light Harvesting, Chemical Energy Conversion and Fuel Generation
Research on solar fuels accelerated dramatically when Fujishima and Honda190 demonstrated that water photochemically splits into hydrogen and oxygen at titanium dioxide (TiO2) photo- electrodes illuminated with sunlight. The findings presented both enormous opportunities and challenges: TiO2is both cheap and chemically durable, making it appealing as a photocatalyst and photoelectrode material, but the efficiency of sunlight-driven water splitting at unmodified TiO2 is poor. The two most common polymorphs of TiO2, rutile and anatase, both require excitation with ultraviolet (UV) light to create excited state electron–hole pairs that drive photochemical reactions (Fig. 7). UV light comprises < 5% of the terrestrial solar spectrum.
Immeasurable effort has been exerted to improve the utilization of both UV and visible light
Fig. 7 Schematic representation of photocatalysis at (a) dispersed semiconductor materials; and (b) in a photoelectrochemical water-splitting cell.
by sensitizing TiO2with dyes, atomic dopants, plasmonic metal nanoparticles, and semiconduc- tor nanocrystals, as well as by rendering it as high surface area nanostructured materials and nanoparticles.191–193 Visible light active photocatalysts derived from semiconductors with narrower bandgaps have also been extensively investigated.194–196
Photocatalysis at dispersed semiconductor powders [Fig.7(a)] or semiconductor photoelectr- odes [Fig.7(b)] requires that the semiconductor absorbs a sufficiently energetic photon to pro- mote an electron from the valence band (VB) to the conduction band (CB) of the semiconductor (step 1). After creation of the electron–hole pair, the CB electron and VB hole must each diffuse to the semiconductor surface (step 2) before the electron–hole pairs relax via recombination pathways, removing them from the photochemical process (step 3).
Upon reaching the semiconductor surface, the electron and hole react (step 4) to reduce the electron acceptor molecules (A) and oxidize the electron donor molecules (D). In photocatalytic water splitting, H2O acts as the electron donor and is split into oxygen and protons (Hþ), while transferring the electrons to the semiconductor [Eq. (1)]. Protons are reduced by the CB electrons of the semiconductor to yield molecular hydrogen [Eq. (2)]:
2H2O → 4Hþþ 4e−þ O2; (1)
4Hþþ 4e−→ 2H2: (2)
Several recent reviews extensively describe the various approaches to achieving photocata- lytic water splitting.197–205Because both the photocatalytic oxidation step [Eq. (1)] and reduction step [Eq. (2)] are catalytically challenging in pure water, the activity of new oxidation or reduc- tion cocatalysts (typically either catalytic noble metal nanoparticles or molecules attached to the semiconductor surface) for the individual half reactions are typically studied in isolation. To evaluate hydrogen generation kinetics [Eq. (2)], an easily oxidized sacrificial electron donor, such as methanol, is often added to the reaction to remove the kinetic bottleneck comprising water oxidation [Eq. (1)]; when evaluating oxidative water splitting, an electron acceptor is added to the reaction to remove the effects of slow hydrogen generation kinetics, especially in neutral or basic conditions, when proton concentration is low.
Typical values for apparent QE for H2-generation via visible light driven photocatalytic split- ting of H2O are < 1%,197with the notable exception of the work by Domen and coworkers, who report QE of 2.5% with gallium nitride/zinc oxide modified with rhodium chromate,206and zinc- germanium oxynitride semiconductor materials modified with ruthenium oxide207cocatalysts.
The reason that photocatalytic efficiency for water splitting in pure H2O using visible light remains generally poor is that very few photocatalysts perform all of the steps depicted in Fig. 7well enough to successfully execute the entire process efficiently.
2.3.1 Tandem photoelectrochemical/photovoltaic devices for water splitting The often orthogonal requirements for good light-harvesting efficiency, charge separation, and catalytic reaction efficiency suggest that unburdening the catalytic material from at least one of these steps could enable solar fuel processes to run more efficiently. Khaselev and Turner208 developed a tandem PEC/PV system that separated the light harvesting and photovoltage gen- eration from the catalytic water oxidation processes (while still driving reductive hydrogen gen- eration at the photoelectrode). The energy efficiency for H2-generation under simulated sunlight—defined as the ratio of the energy value of H2produced to the total energy of absorbed light—was 12.4%. The practical drawback of their device (Fig.8) is that the PV element was an expensive, epitaxially grown n–p–n GaAs/GaAs/GaInP device. In the same year, Rocheleau et al.209 described a tandem PEC/PV system using cheaper amorphous silicon as the active material in the triple-junction PV and reported solar-to-H2 efficiencies of 7.5% to 7.8%.
Very recently, Cox et al.210demonstrated 10% solar-to-H2efficiency with tandem PEC/PV devi- ces using inexpensive commercial solar cells based on crystalline Si on the PV side and low-cost hydrogen and oxygen generation catalysts in the PEC. This tandem approach coupled with state- of-the-art nonprecious catalyst materials has been dubbed the artificial leaf.211
Given the much higher efficiencies for solar H2-generation from water achieved at tandem PEC/PV devices (> 10% solar-to-H2 energy efficiency under simulated sunlight) compared to those measured for dispersed photocatalysts illuminated with visible light (typically < 1% QE, which translates into still lower solar-to-H2energy efficiency), the question arises as to whether solar fuels photochemistry at dispersed photocatalysts has already lost the technological race. As the price of PV devices decreases, the tandem approach becomes increasingly attractive.
However, dispersed semiconductor nanomaterials can separate electrons and holes extremely rapidly, and if durable, cost-effective means of improving the efficiency of the cheapest semi- conductor photocatalyst materials, such as TiO2and iron oxides, are discovered, dispersed pho- tocatalytic materials could conceivably emerge as the more cost-effective technologies.
2.3.2 Liquid fuel production via photocatalytic CO2 reduction
While the recent advances in H2-generation photocatalysis are tremendously important, the infrastructure for storing and using H2 as a use-flexible fuel supply still does not exist. In the near term, liquid fuels will continue to comprise a substantial portion of the world fuel sup- ply, particularly in the transportation sector. The photocatalytic reduction of CO2 to fuels and fuel precursors is still more difficult than photocatalytic water splitting. The photochemistry follows the same general pathway outlined in Fig.7(a), with the final reduction step [Fig.7(a), step 4a] being the slow, inefficient reduction of CO2to the most desired products, either CH4or CH3OH. Side products—wanted or unwanted—typically include a mixture of H2, CO, and Fig. 8 (a) Schematic of the monolithic PEC/PV device. (b) Idealized energy level diagram for the monolithic PEC/PV photoelectrolysis device. (Reproduced with permission from Ref. 208.
HCOOH. If photocatalytic CO2reduction is also truly to be carbon-neutral, the initial oxidation chemistry (step 4b) should use H2O as the electron donor. In short, photocatalytic CO2reduction involves all of the difficult steps of photocatalytic water splitting, with a particularly onerous reduction step added at the end of the catalytic process.
Like catalysts for photochemical water splitting, photocatalytic CO2reduction and semicon- ductor-based photocatalysts have been extensively reviewed in the past few years.212–217 Considerable effort has been focused on both TiO2-based photocatalysts212,216and on alternative semiconductors to TiO2.214 An impressive QE for photocatalytic CO2 reduction has been achieved when using UV light: Inoue et al.218reported 32.5% QE for the reduction of CO2in aqueous bicarbonate to HCOOH at Cd-modified ZnS microcrystals illuminated at 280 nm;
Tseng and coworkers achieved QE of 10% for photoreduction of CO2 at sol–gel derived Cu-modified TiO2 illuminated at 254 nm in aqueous base;219 while Slamet et al.220reported photocatalytic reduction of CO2to CH3OH at UV-illuminated copper oxide doped TiO2nano- crystals in aqueous bicarbonate with QE ¼ 19.2%. Visible light photocatalytic CO2reduction is still considerably less efficient: Sato et al.221reported 1.9% QE for photocatalytic conversion of CO2 to mixtures of CO, HCOOH, and H2 at nitrogen-doped Ta2O5 modified with ruthenium polypyridyl cocatalysts. Typical QEs for the photocatalytic reduction of CO2 to CH3OH and CH4using visible light are even lower:∼0.02% to 0.2%.222–224Though the efficiencies achieved with visible light illumination are low, the high QE achieved under UV light suggests that the CO2reduction bottleneck in the catalytic cycle is not necessarily prohibitive to making visible light photocatalytic CO2 reduction technologically viable. As is the case with visible light photocatalytic water splitting, the success of the CO2pathway will strongly depend on the right semiconductor design or sensitization scheme to efficiently produce reactive electron–hole pairs under visible illumination.
2.3.3 Application of nanophotonics to solar fuels photocatalysis:
photonic crystals for enhanced light harvesting
Research in the past decade has demonstrated that photocatalytic materials either incorporated into or expressed directly as PCs are∼2× to 3× more active than the standard nanostructured forms of the same materials, regardless of the choice of semiconductor photocatalyst. Several illustrative examples will be specifically described below. PCs are periodic structures with alter- nating phases of high- and low refractive index materials in one, two, or three dimensions.225–228 Radiation of wavelengths comparable to the PC feature dimensions is diffracted according to a modified version of Bragg’s law (fitted to the geometry and refractive indices of the phases in the PC). The most strongly diffracted wavelengths cannot propagate in the PC structure; the wave- length at the center of this distribution is known as the stop band, or photonic bandgap. PCs enhance light absorption in the semiconductor via the slow photon effect. Photons with energies slightly higher and lower than the stop band are substantially slowed, with light frequencies at the low-energy (red) edge of the stop band localized and multiply scattered in the higher dielectric part of the PC; those at the high-energy (blue) edge are multiply scattered within the low-index portion.229In semiconductor photocatalysis, the slow photon effect enables greater interaction of the slowed photons with the semiconductor or sensitizer, improving the probability of their absorption.
The most frequently applied PC geometry in photocatalysis, depicted in Fig.9, is the inverse opal,230which is relatively simple to fabricate and allows control of feature dimensions, enabling tuning of the stop band. Inverse opals are commonly synthesized by infiltrating a colloidal array of carboxylate-modified polystyrene spheres with metal oxide precursor solutions followed by subsequent removal of the colloidal array and calcination.231–233
2.3.4 Hydrogen generation by photocatalysis at TiO2 photonic crystals
Liu et al.235employed a series of TiO2PC films modified with Pt nanoparticles with stop bands ranging from 307 to 434 nm in photocatalytic hydrogen generation experiments and observed enhancement of photocatalytic activity relative to Pt∕TiO2 control materials that were not
incorporated into PC structures. The largest enhancement factors (EFs) under white light illu- mination occurred for PC films with stop bands of 307 nm (EF ¼ 2.4) and 342 nm (EF ¼ 2.5).
Semiconductor photocatalysts sensitized to visible light are also readily adaptable for PC-based enhancement of photocatalytic activity. For example, modification of TiO2with surface plasmon resonance (SPR) active gold (Au) nanoparticles has recently emerged as a viable strategy for enhancing visible light absorption.236–239PEC water splitting at TiO2PCs modified with 10-nm Au nanoparticles was enhanced by a factor of 2 relative to Au-modified nanocrystalline (but nonphotonic) TiO2 films.240 Alternative materials to TiO2 for photocatalytic water split- ting194–196 also benefit from PC-enabled improvement of light utilization. The inverse opal PC design has been applied to photocatalytic iron oxides,241 tungsten oxide,242,243and binary oxides.234,244,245 Enhancement of water-splitting photocatalytic activity is consistently two to three times higher than that of the non-PC control materials.
Light-scattering structures more complex than inverse opals also enhance water-splitting photocatalysis. Because the more complex structures are imperfectly periodic or aperiodic over the length of the light scattering layer, photocatalytic enhancement derives from disorgan- ized internal scattering of photons rather than by slow photon effects. Templated TiO2replicas of butterfly wings, modified with Pt nanoparticles and featuring semiordered arrays of holes and inverted ridges, enhanced photocatalytic water splitting 2.3× compared to that at nonphotonic Pt-modified TiO2.246 Similarly, porous TiO2 structures templated from leaves exhibited enhanced light absorption and H2-generation enhancement.247
2.4 Optical and Photonic Sensors for Energy Harvesting and Power Production Optical and photonic sensors are commonplace for a wide variety of applications in the broad field of energy. In this section, their specific use in three very different applications relating to energy harvesting and the production of power will be presented, namely solar thermal and PV systems, the oil and gas industries, and wind turbines.
Fig. 9 SEM of (a) colloidal crystal template of polystyrene spheres (200 nm) and (b) three-dimen- sional ordered macromesoporous architecture of Mo∶BiVO4. (Reproduced with permission from Ref.234. Copyright ACS.)
2.4.1 Sun-tracking systems
The output power of solar thermal and PV systems can be maximized by the use of sun-tracking systems, defined as electromechanical devices for orienting the solar energy systems toward the sun. Given that the diurnal and seasonal movement of the earth affects the radiation intensity on any solar energy system,248sun-tracking devices are used to determine with a high degree of accuracy the position of the sun throughout the course of the day on a yearly basis. As such, sun trackers are in charge of moving the solar energy systems to compensate for the motion of the earth, aiming at keeping the best orientation relative to the sun, i.e., perpendicular to solar radiation. The use of sun trackers has the potential to increase the collected energy by 10% to 100%, depending on many factors including the time of the year and the geographical position. In the particular case of concentrator applications for PVs and solar thermal applica- tions, tracking systems are essential because concentrators do not produce energy unless pointed at the sun.
Solar tracking can be active or passive and can be implemented as one- or two-axis sys- tems.249Single-axis trackers follow the sun’s apparent east-to-west movement, while dual-axis trackers also tilt the solar collector or module to follow the sun’s altitude angle.250Figure10(a) shows schematic diagrams of the operation of single- and dual-axis tracking systems, while Fig.10(b)illustrates a prototype of a dual-axis tracking system, comprising two stepper motors, a control circuit board and drivers, reducing gears, a sun positioning device (photodiode array), a global positioning system module, and fibers. Commercially, tracking systems are available in either a single-axis or a dual-axis design.
Active trackers can be classified as either open-loop or closed-loop types,249depending on their mode of signal operation. Succinctly, an open-loop type of controller computes its input into a system using only the current state and the algorithm of the system and without using feedback to determine if its input has achieved the desired goal (i.e., algorithm-based).
Closed-loop types of sun-tracking systems are based on feedback control principles. In these systems, a number of inputs are transferred to a controller from sensors, which detect relevant parameters induced by the sun, manipulated in the controller and then yield outputs (i.e., sensor-based).
Fig. 10 Schematic diagrams of different solar trackers: (a) dual-axis tracker, (b) polar aligned sin- gle-axis tracker, and (c) horizontal single-axis tracker. (Reproduced from Ref.251). Lower panel:
Prototype of a dual-axis sun tracking system and concentrated sunlight transmission system via fibers. (Reproduced from Ref.252.)